# measured by inelastic neutron scattering

Post on 23-Dec-2016

216 views

Embed Size (px)

TRANSCRIPT

PHYSICAL REVIEW B 83, 214519 (2011)

Itinerant spin excitations in SrFe2As2 measured by inelastic neutron scattering

R. A. Ewings,1,* T. G. Perring,1,2 J. Gillett,3 S. D. Das,3 S. E. Sebastian,3 A. E. Taylor,4 T. Guidi,1 and A. T. Boothroyd41ISIS Facility, STFC Rutherford Appleton Laboratory, Chilton, Didcot, Oxon OX11 0QX, United Kingdom

2Department of Physics and Astronomy, University College London, Gower Street, London WC1E 6BT, United Kingdom3Cavendish Laboratory, University of Cambridge, JJ Thomson Avenue, Cambridge CB3 0HE, United Kingdom

4Department of Physics, University of Oxford, Clarendon Laboratory, Parks Road, Oxford OX1 3PU, United Kingdom(Received 20 April 2011; published 15 June 2011)

We report inelastic neutron-scattering measurements of the magnetic excitations in SrFe2As2, the parent ofa family of iron-based superconductors. The data extend throughout the Brillouin zone and up to energies of260 meV. The spectrum calculated from a J1-J2 model does not accurately describe our data, and we showthat some of the qualitative features that the model fails to describe are readily explained by calculations froma five-band itinerant mean-field model. In particular, the high-energy part of the spectra recorded above TN donot differ significantly from those at low temperature, which is explained by the itinerant model and which hasimplications for theories of electronic nematic and orbital ordering.

DOI: 10.1103/PhysRevB.83.214519 PACS number(s): 74.25.Ha, 74.70.Xa, 75.30.Ds, 78.70.Nx

I. INTRODUCTION

The new iron-based superconductors show an in-triguing interplay between structure, magnetism, andsuperconductivity.13 It is likely that the paradigm to under-stand these materials will be rather different from that used toapproach the cuprate superconductors, since the parent com-pounds for iron-based superconductors are bad metals, ratherthan Mott insulators. Theoretical estimates suggest that theelectron-phonon interaction is not the primary component ofthe pairing interaction in the iron-based superconductors,4 andmost attention is now on magnetic pairing mechanisms.5 Muchtheoretical and experimental effort has therefore been devotedto understanding the magnetism in this family of materials.6 Akey issue is whether the magnetism is better described withina weak-coupling (itinerant)7 or strong-coupling (localized)8picture.

One of the most direct ways to identify the character ofthe magnetism is to study the magnetic excitation spectrumby inelastic neutron scattering (INS). Previous INS measure-ments of the antiferromagnetic (AFM) 122-arsenidesXFe2As2(where X is an alkali-earth metal) have been interpreted interms of linear spin-wave theory, predicated on local-momentJ1-J2 models.911 These models include nearest-neighbor(J1) and in-plane diagonal next-nearest-neighbor (J2) Fe-Feexchange interactions. A particularly interesting result fromthis approach when applied to CaFe2As2 is the very largedifference between J1a and J1b, the two in-plane nearest-neighbor exchange parameters.11 Various mechanisms havebeen proposed to explain this anisotropy, including electronicnematic ordering,12 orbital ordering,13 and the crystal structureitself.14 An important piece of information, lacking up tonow, is whether the anisotropy is modified on warming abovethe combined magnetic and structural transition temperature(TN,s), i.e., how the magnetic spectrum is modified on thechange of symmetry between low-temperature orthorhombicand high-temperature tetragonal phases. Recent resistivitymeasurements of detwinned samples of Ba(Fe1xCox)2As2show that there exists a large electronic anisotropy that persistsabove TN,s.15 Previous INS measurements of CaFe2As2 aboveTN,s (Ref. 16) probed excitations only up to 60 meV. Given

the possible role of magnetic fluctuations in the origin ofthe superconductivity of iron pnictides, further data on themagnetic spectrum in the tetragonal phase are of great interest.

The questions we set out to answer here are, first, arethe magnetic interactions in SrFe2As2 anisotropic in theordered state, as in other 122-arsenides; second, do the spinexcitation spectra change significantly on warming aboveTN,s; and third, how robust is the local-moment description ofthe INS spectra? The INS results we describe here probe themagnetic excitations throughout the Brillouin zone (BZ) overthe energy range 5 < E < 260 meV, below and above TN,s.We find that within a localized model the magnetic exchangeparameters are strongly anisotropic below and above TN,s, andthat an itinerant model gives the better qualitative descriptionof the data. The form of the data is not significantly altered onwarming above TN,s.

II. EXPERIMENTAL DETAILS

Single crystals of SrFe2As2 were grown by the self-fluxmethod.17,18 The crystals are highly homogeneous, as verifiedby microprobe analysis, a well-defined magnetic-structuraltransition temperature of TN,s = 192 K, and by the observationof quantum oscillations from samples from the same growth.18

On cooling through TN,s, the crystal symmetry changesfrom I4/mmm to Fmmm, and an AFM structure developswith propagation vector QAFM = (0.5,0.5,1) referring to theI4/mmm unit cell [wave vectors are given in reciprocal-latticeunits (rlu)]. As the magnetic dynamics in SrFe2As2 arerelatively two dimensional we will henceforth give only in-plane wave-vector components. Further, from now on we indexwave vectors with respect to the square unit cell formed bythe Fe atoms in the paramagnetic phase (aFe = bFe = 2.8 A).In this convention QAFM = (0.5,0). The unit cells and theircorresponding Brillouin zones are shown in Fig. 1.

The INS experiments were performed on the MER-LIN time-of-flight (TOF) chopper spectrometer at the ISISfacility.19 Twenty-one single crystals were co-aligned to givea mosaic sample of mass 5.4 g, with a uniform mosaic of4 (full width at half maximum). Spectra were recorded at

214519-11098-0121/2011/83(21)/214519(6) 2011 American Physical Society

R. A. EWINGS et al. PHYSICAL REVIEW B 83, 214519 (2011)

FIG. 1. (Color online) (a) Projection of the real-space crystalstructure onto the ab plane, with As atoms omitted for clarity. Thesolid (black) square is the unit cell of the Fe sublattice, the dashed(blue) square is the orthorhombic unit cell (space group Fmmm),and the dotted (red) diamond is the tetragonal I4/mmm unit cell.(b) Corresponding Brillouin zones. Referring to the Fe sublattice, thestandard square-lattice symmetry points are = (0,0), X = (0.5,0),and M = (0.5,0.5), and X is the AFM ordering wave vector. Thearrows labeled and indicate the direction of one-dimensional(1D) cuts and 2D slices shown in Figs. 2 and 3.

temperatures of 6,212 (TN,s + 20 K), and 300 K with neutronsof incident energy Ei = 50, 100, 180, 300, and 450 meV. Thesample was aligned with the c axis parallel to the incidentneutron beam, and the a axis horizontal. Data from equivalentpositions in reciprocal space were averaged to improvestatistics. The scattering from a standard vanadium samplewas used to normalize the spectra, S(Q,E), and place them onan absolute intensity scale, with units mb sr1 meV1 f.u.1,where 1 mb = 1031 m2 and f.u. stands for formula unit ofSrFe2As2.

III. RESULTS AND ANALYSIS

The general form of the scattering at T = 6 K TN,s isillustrated by the energy-momentum slice in Fig. 2(a). Themagnetic spectrum is similar to that of CaFe2As2,10,11 withintensity dispersing out of the QAFM positions. The dispersionis revealed in more detail in Fig. 3, which presents wave vectorscans at four different energies. A single peak centered onQAFM = (0.5,0) at low energies develops into a pair of peaksat 75 meV, which continue to separate and broaden withincreasing energy. These peaks converge on Q = (0.5,0.5)at E 230 meV. Figures 2(b) and 2(c) show that at T =212 K > TN,s and T = 300 K TN,s the spectrum remainsvery similar to that of the ordered state, which means thatstrong AFM correlations persist well into the paramagneticphase.

Figure 4 provides a comparison of the spectra recorded at6, 212, and 300 K for wave vectors near (0.5,0) and (0.5,0.5).The signals at 212 and 300 K are somewhat broader than that at6 K, but otherwise there are no marked differences associatedwith the change of crystal structure, even well above TN,s.

We first compare the data with the linear spin-wave spec-trum calculated from a local-moment Heisenberg Hamiltonian.This model is the standard one used to interpret the spinexcitations in the parent 122 compounds,911 and is describedin detail in the Appendix. The key exchange parameters in thismodel are J1a , J1b, and J2, which define the exchange along

FIG. 2. (Color online) Energywave-vector slices through theINS datasets at (a) T = 6 K, (b) T = 212 K, and (c) T = 300 K.Panels (d) and (e) show simulations of the spectrum over the same Qand energy range using a local-moment spin-wave model with J1a =J1b, J1b < 0, and J1a = J1b, respectively. Panels (f) and (g) showthe calculated (Q,E) for the AFM phase and the paramagneticphase, respectively; both taken from Ref. 27, and convoluted withthe instrumental resolution, with the energy rescaled by a factor0.85. Data are from the run with Ei = 450 meV, and the intensityof both data and simulations have been multiplied by E to improveclarity. The Fe form factor has been included in the simulations.Dashed lines in panels (d) and (e) indicate the simulated dispersionrelations for the high-energy parameters (see caption to Fig. 3) and forJ1a = J1b, respectively. Dashed lines in panels (f) and (g) are the lociof maximum intensity for the calculated (Q,E). (The calculatedlow-energy incommensurate behavior in (g) is discussed in Ref. 27and likely arises from limitations of the model. See text for furtherdiscussion of this point.)

the a and b directions and the ab diagonal, respectively, aswell as interplanar exchange Jc.

To fit data of the type presented we incorporated theresolution of the spectrometer in (Q,E) space, since the widthsof peaks in the scattering are often very strongly coupled tothe instrumental resolution, which is itself a function of Ei.We used the TOBYFIT software,20 which uses Monte Carlomethods to account for the effects of the (Q,E) resolution ofTOF spectrometers. We fitted the measured scattering crosssection, in the form of a set of one-dimensional cuts, overthe entire energy range for which magnetic excitations wereextant, convoluting the cross section with the spectrometerresolution.

Neutron inelastic-scattering measurements of SrFe2As2performed on a triple-axis spectrometer with relatively low-energy transfers21 reveal a single gap of 6.5 meV in theexcitation spectrum. There is no evidence for two gaps, sowe set the two modes described by Eq. (A2) in the Appendixto be degenerate, i.e., C = 0 in Eq. (A3) and the in-planeand out-of-plane single-ion anisotropy terms are equal (Kab =Kc = K). The single-ion anisotropy terms are thus determinedby the size of the gap , which is given by

2

16S2= K2 + [J1a + 2J2 + Jc]K. (1)

214519-2

ITINERANT SPIN EXCITATIONS IN SrFe2As2 . . . PHYSICAL REVIEW B 83, 214519 (2011)

0.25 0 0.25 0.50.6

0.8

1

1.2

1.4

1.6

(0.5K,0.5+K) [r.l.u.]

160

R. A. EWINGS et al. PHYSICAL REVIEW B 83, 214519 (2011)

existence of an electronic nematic state has recently beenproposed to explain anisotropy in the in-plane resistivity15and elastic properties25 of iron pnictides. In some cases theelectronic nematic order is predicted to persist above TN,s,12although by only a few degrees at most. Thus any evidence ofbroken symmetry above TN,s is unlikely to be due to nematicorder directly, but could perhaps be ascribed to nematiclikefluctuations, as in Ref. 25, in which it is suggested that nematicfluctuations might persist up to room temperature. Our highertemperature measurements were performed at both 20 K aboveTN and room temperature, and as can be seen in Figs. 2(b) and2(c), and Fig. 4, the neutron-scattering spectra are very similar.Although one might expect some change in the spectra oversuch a wide temperature range, we cannot completely rule outthe existence of nematic fluctuations.

Orbital ordering has also been suggested to explain theanisotropy.13 In this case it has been predicted that a spin-wavemode would exist at high energies at Q = (0.5,0.5). Thesame calculations also indicate that on warming the energyof this mode softens slightly, and the peak height of thedynamical response function S (Q,E) decreases rapidly. Thebroadening and lack of appreciable softening of the mode atQ = (0.5,0.5) agree well with our data. However, as shown inFigs. 4(c)4(e), the peak intensity is essentially unchanged, atvariance with the calculation. Note that in Ref. 13 the orbitalorder parameter is treated as an Ising-like parameter, so itis possible that if one considered instead a case in whichthere was partial orbital polarization the form of S(Q,E)vs temperature may be altered.

If the local-moment model cannot be reconciled withour data, as seems likely, then what about itinerant-electronmodels,26,27 or hybrid models that combine both local mo-ments and itinerant electrons?28 In order to capture the keyfeatures of the data it is likely that a relatively detailedmodel will be required. Indeed, a comparison of the calculated (Q,E) from a minimal band model26 shows that it doesnot provide a good description of our data, except for 50 meV.

However, a mean-field model based on a more realistic five-band structure27 appears to give quantitatively good agreementwith some of the features observed here. We illustrate thisin Figs. 2(a) and 2(f), which show the low-temperature INSdata together with the calculated dynamical susceptibility (Q,E), convoluted with our instrumental resolution. Wealso over-plot the locus of maximum intensity from the itin-erant model calculation. This curve is rather more structuredthan the smooth dispersion curves shown in Figs. 2(d) and2(e), with several abrupt changes of gradient, which wouldof course be parametrized in a local-moment treatment byexchange parameters that changed with energy. The energyscale of the calculated (Q,E) has been changed by a factor0.85 compared to the published calculation. This rescalingis likely due to the fact that in a mean-field approximationthe energy scale typically needs to be renormalized downdue to correlation effects not included in the model. Thecalculations in Ref. 27 were performed with a Coulombinteraction U = 1.2 eV and Hund coupling J = 0.22 eV,chosen to yield the observed ordered moment of 0.8B. Therehas, however, been some debate as to the strength of the

electron correlations, as characterized by U and J , in ironpnictides.2931

Fine tuning of the model parameters, i.e., U and J , wouldno doubt improve the description of the data, but the presentset seems to work reasonably well. Thus the spin fluctuationspectrum of SrFe2As2 that we measured indicates that this122-arsenide exhibits rather weak electron correlations. Inaddition we note that the calculat...